Physica B 284}288 (2000) 939 } 940
Ultrafast dynamics in Pr-doped and oxygen-de"cient YBCO "lms by femtosecond spectroscopy K.H. Wu*, C.W. Luo, J.Y. Juang, T.M. Uen, Y.S. Gou Department of Electrophysics, National Chiao Tung University, Hsinchu, Taiwan, Republic of China
Abstract We have systematically measured the transient re#ectivity (*R/R) in Pr-doped YBCO (Pr Y Ba Cu O ) and V \V partially oxygen de"cient YBCO (YBa Cu O ) thin "lms at temperatures ranging from 300 to 12 K by using the \B femtosecond pump}probe technique. Measurements performed at low temperatures indicate that the magnitude, polarity, and relaxation time of the transient re#ectivity is strongly dependent on the photon energy and pumping intensity of the optical excitation, the ambient temperature, and the doping level of the superconducting thin "lms. Moreover, the temperature dependence of the Fermi-level position was also observed. 2000 Elsevier Science B.V. All rights reserved. Keywords: Femtosecond laser; Oxygen de"ciency; YBaCuO substituted; Ultrafast dynamics
The ultrafast optical response, dealing with the role of electrons, phonons, and their interaction and the dynamics of charge carriers in either normal or superconducting state, is particularly important to study the physical properties of high-¹ superconductors (HTSCs). However, for femtosecond pump-probe experiments at temperatures near ¹ , *R/R may contain more complic ated nonequilibrium dynamics [1,2]. The abrupt change of the density of states near the Fermi level, the photogeneration and relaxation of quasiparticles, and the opening of the superconducting gap or pseudogap  may all come into play simultaneously. Therefore, the relationship between the optical response and the nature of the nonequilibrium superconducting dynamics has not been clearly elucidated in this regime. It is suggestive that, further femtosecond-spectroscopy measurement using the pump and probe beams with di!erent photon energies might be needed to reveal more information about the optical response and the band structure of HTSCs. The Pr Y Ba Cu O "lms with x"0, 0.1, V \V 0.2, 0.3, 0.4, 0.5, 0.6, 0.8, and 1.0 were prepared on (100) LaAlO substrates using pulsed laser deposition. In * Corresponding author. E-mail address: [email protected]
comparsion, the oxygen stoichiometry of a sole YBa Cu O "lm was controlled to vary d (d"0.05, \B 0.1, 0.2, 0.3, 0.4, 0.5, 0.55,(0.6) in a precise and reproducible fashion . The pump}probe measurements used a mode-locked Ti}sapphire laser operating at 775 nm (1.55 eV) which produced a 85 MHz train of 150 fs pulses. The temperature-dependent *R/R curves of YBa Cu O and Pr Y Ba Cu O samples have \B V \V been systematically measured. It is found that the sign of *R always remains positive in the whole temperature range for samples with d)0.2 or x)0.1. On the other hand, for samples with d"0.3 (Fig. 1(a)) or x"0.2 (Fig. 1(b)) and 0.3, the sign of *R is positive when the temperature is larger than ¹ and change gradually to negative when the temperature is lowered than ¹ !*¹, where *¹ is the increase in temperature due to laser pulse. For samples with d'0.5 or x'0.5, the sign of *R becomes negative in the whole temperature range. However, for the "lms with d)0.2 or x)0.1, the present results are quite di!erent from those reported previously  where higher photon energy (&2.0 eV) was used and larger, negative *R was obtained when ¹(¹ . This implies that other mechanisms may have contributed to the negative component of measured *R if the probe energy is near the position of Fermi level relative to the Cu upper Hubbard band UHB (E ). Indeed, as is evident
0921-4526/00/$ - see front matter 2000 Elsevier Science B.V. All rights reserved. PII: S 0 9 2 1 - 4 5 2 6 ( 9 9 ) 0 2 2 5 8 - 9
K.H. Wu et al. / Physica B 284}288 (2000) 939}940
Fig. 1. The temperature dependence of the transient *R/R curves for (a) YBa Cu O "lm (¹ "61 K) and (b) Pr Y Ba Cu O "lm (¹ "69 K). The average pump power was 10 mW and probe beam was 2 mW.
Fig. 3. The temperature dependence of the transient *R/R curves for a nonsuperconducting PrBa Cu O "lm. The aver age pump power was 30 mW and probe power was 2 mW.
*R was positive while the pump power was reduced to 10 mW, it became negative. Moreover, Fig. 3 SHOWS THAT THE SIGN reversal of *R also occurred when the ambient temperature was cooled to below 233 K. The change of *R sign in both cases can be interpreted as the temperature dependence of the Fermi-level shift . It is measurable especially when the Fermi temperature is low (&10 K) for the insulating "lms. In principle, the temperature dependence of the Fermi-level position can be determined by the time-resolved *R/R measurement provided that the probe energy can be tuned over a wide range. Fig. 2. The transient *R/R curves at room temperature for PrBa Cu O "lm. The average pump power was (a) 20 mW and (b) 10 mW.
from Fig. 1, when the probing photon energy (1.55 eV in our case) was near E , the sign of *R was reversed at ¹(¹ . for samples with d"0.3 or x"0.2. It is noted that in nonsuperconducting "lm, such as Pr Y Ba Cu O "lm with x'0.6 or YBa Cu O V \V \B "lm with d'0.6, the sign of *R were strongly related to the pumping intensity and the ambient temperature. As shown in Fig. 2, when a PrBa Cu O "lm was illuminated by a pumping power of 20 mW, the sign of
Acknowledgements This work was supported by the National Science Council of Taiwan, R.O.C. under grants: NSC88-2112M009-019.
References    
D.H. Reitze et al., Phys. Rev. B 46 (1992) 14 309. J. Demsar et al., Phys. Rev. B, to be published. K.H. Wu et al., Jpn. J. Appl. Phys. 37 (1998) 4346. L. Shi et al., Appl. Phys. Lett. 64 (1994) 1150.